Guest Tunable Structure and Spin Crossover Properties in a Nanoporous Coordination Framework Material
Suzanne M. Neville; Gregory J. Halder; Karena W. Chapman; Martin B. Duriska; Boujemaa Moubaraki; Keith S. Murray; Cameron J. Kepert; Journal of the American Chemical Society 131 (2009) 12106–12108; doi:10.1021/ja905360g

data_4104952
_publ_contact_author_address
; 
School of Chemistry
University of Sydney
NSW 2006
Australia
;
_publ_contact_author_email       c.kepert@chem.usyd.edu.au
_publ_contact_author_fax         +61-2-9351-3329
_publ_contact_author_name        'Prof. Cameron J. Kepert'
_publ_contact_author_phone       +61-2-9351-5741
_publ_section_title
;
 Guest Tunable Structure and Spin Crossover Properties in a Nanoporous
 Coordination Framework Material
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              12106
_journal_page_last               12108
_journal_paper_doi               10.1021/ja905360g
_journal_volume                  131
_journal_year                    2009
_chemical_formula_moiety         'C30 H32 Fe N6 O4 S2, 3(C2 O)'
_chemical_formula_sum            'C36 H32 Fe N6 O7 S2'
_chemical_formula_weight         780.65
_chemical_name_common            SCOF-2(Et)as
_space_group_IT_number           130
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  '-P 4a 2ac'
_symmetry_space_group_name_H-M   'P 4/n c c :2'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   14.639(5)
_cell_length_b                   14.639(5)
_cell_length_c                   17.851(12)
_cell_measurement_reflns_used    111
_cell_measurement_temperature    200(2)
_cell_measurement_theta_max      16.183
_cell_measurement_theta_min      2.783
_cell_volume                     3825(3)
_computing_cell_refinement       'SMART (BrukerAXS, 1997)'
_computing_data_collection       'SMART (BrukerAXS, 1997)'
_computing_data_reduction        'SAINT+ (BrukerAXS, 1997)'
_computing_molecular_graphics    'XPMA/ZORTEP, WebLab Viewer 3.7'
_computing_publication_material  XCIF
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      200(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Bruker SMART 1000'
_diffrn_measurement_method       \w
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0000
_diffrn_reflns_av_sigmaI/netI    0.0715
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            903
_diffrn_reflns_theta_full        20.01
_diffrn_reflns_theta_max         20.01
_diffrn_reflns_theta_min         1.97
_diffrn_standards_decay_%        0
_diffrn_standards_interval_count 0
_diffrn_standards_interval_time  0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    0.558
_exptl_absorpt_correction_T_max  0.8732
_exptl_absorpt_correction_T_min  0.8595
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   sadabs
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    1.355
_exptl_crystal_description       rod
_exptl_crystal_F_000             1616
_exptl_crystal_size_max          0.28
_exptl_crystal_size_mid          0.25
_exptl_crystal_size_min          0.25
_refine_diff_density_max         0.539
_refine_diff_density_min         -0.856
_refine_diff_density_rms         0.113
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.133
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     120
_refine_ls_number_reflns         903
_refine_ls_number_restraints     16
_refine_ls_restrained_S_all      1.144
_refine_ls_R_factor_all          0.1918
_refine_ls_R_factor_gt           0.0880
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.1565P)^2^+66.8279P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2308
_refine_ls_wR_factor_ref         0.3644
_reflns_number_gt                443
_reflns_number_total             903
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ja905360g_si_001_3.cif
_cod_data_source_block           SCOF-2(Et)as
_cod_original_sg_symbol_H-M      'P 4/n c c'
_cod_database_code               4104952